# Recent Progress of Fabrication of Cell Scaffold by Electrospinning Technique for Articular Cartilage Tissue Engineering

Authors: Yingge Zhou; Joanna Chyu; Mimi Zumwalt
Journal: International Journal of Biomaterials
 (2018)

---

## Abstract

As a versatile nanofiber manufacturing technique, electrospinning has been widely employed for the fabrication of tissue engineering scaffolds. Since the structure of natural extracellular matrices varies substantially in different tissues, there has been growing awareness of the fact that the hierarchical 3D structure of scaffolds may affect intercellular interactions, material transportation, fluid flow, environmental stimulation, and so forth. Physical blending of the synthetic and natural polymers to form composite materials better mimics the composition and mechanical properties of natural tissues. Scaffolds with element gradient, such as growth factor gradient, have demonstrated good potentials to promote heterogeneous cell growth and differentiation. Compared to 2D scaffolds with limited thicknesses, 3D scaffolds have superior cell differentiation and development rate. The objective of this review paper is to review and discuss the recent trends of electrospinning strategies for cartilage tissue engineering, particularly the biomimetic, gradient, and 3D scaffolds, along with future prospects of potential clinical applications.


---

## Body

## 1. Introduction

Tissue engineering has emerged as an alternative cell-based approach designed to substitute damaged organs with tissues generatedin vitro. It overcomes the barriers of conventional allograft transplantation, such as the scarcity of donor organs, the complexity of surgery, and complicated postoperative care [1]. In many cases, it involves the utilization of a scaffold, an engineered porous supporting material for tissue regeneration. Scaffolds mimic the extracellular matrix (ECM) of the original tissues and reproduce or replicate the natural tissue environment. In addition, scaffolds can foster certain mechanical and biological properties to modify the behavior of different cell phases [2–4].Articular cartilage is tissue located between bones, which can withstand compressive and shear forces several times that of human body weight for years due to its low friction and high load bearing capacity [5, 6], attributed to the unique composition of its ECM [7]. However, it is also the unique ECM that makes the repair of articular cartilage extremely difficult [8]. The micro fissures caused by repetitive cyclic loading might not be visible to the eye but continuously undermine the integrity of collagen fibrils and proteoglycan network [9], causing cartilage destruction over time and leading to degenerative joint disease or osteoarthritis. Osteoarthritis is no longer common only among the elderly but has extended to the younger population who also need a long-term solution for their painful problem [10].Currently, surgical treatments for knee osteoarthritis include arthroscopic microfracture, Osteoarticular Transfer System (OATS), and autologous chondrocyte implantation (ACI), as well as open procedures such as osteotomy and arthroplasty. Unfortunately, they all fail to provide healthy and vigorous articular cartilage in the long run. For example, osteotomy and arthroplasty can lead to articular exacerbation and impairment of neighboring bones [5]. Cartilage tissue engineering, on the other hand, may provide a potentially better resolution in the treatment of knee osteoarthritis. With scaffolds manufactured especially for articular cartilage, the functional complexity of electrospun scaffolds provides significant advantages over other techniques such as allowing the mesenchymal stem cells to grow in a way that facilitates the formation of fibrous tissue structure. Electrospinning may be a viable approach to achieving highly aligned and biocompatible scaffolds to meet the demands for cartilage tissue engineering.


### 1.1. Electrospinning

An electrospinning system is comprised of at least three units: a high voltage power unit, a material delivery unit (a capillary tube with a small spinneret in general), and a fiber collection unit. A typical electrospinning setup is shown in Figure1 [6]. The randomly distributed nanofibers were collected in Figure 1 on a vertical plate. Usually, an advancement pump is employed to regulate the flow rate of polymeric solution discharged from a syringe. An electrically charged jet of polymer solution or melt is created by a high voltage source. The discharged polymer solution jet goes through an instability process, during which the jet is elongated and the solvent evaporates or solidifies. The jet is finally collected as an interconnected web of ultrathin fibers at the collector that is grounded or connected to an electrode. The diameters of electrospun fibers can range from 10 nm to 100 μm depending on the material, device configuration, and process setup.Figure 1
Typical electrospinning facility with a plate collector [6].Electrospinning is able to generate loosely connected porous mats from submicrometer to nanometer scales in diameter as it is a highly flexible technique to produce continuous fibers. The nanofiber mat yields a high surface area to volume ratio and high porosity [54]. The nanostructure of the mat mimics the structure of the ECM in terms of both morphology and composition [55]. Various patterns of electrospun nanofibers have been fabricated for different biomedical applications ranging from artificial skin to endocrine organs and from the nervous system to cardiovascular tissues [56].


### 1.2. Electrospun Scaffolds for Cartilage Tissue Engineering

Electrospinning as a feasible and versatile technique can manipulate both natural and artificial polymers in nanoscale and promote the proliferation of mesenchymal stem cells (MSCs). Recent research attention has focused on improving the material design of the composition to produce biomimetic, gradient, and 3D scaffolds. Biomimetic scaffold is crucial in the reconstruction of connective tissue such as articular cartilage. Electrospinning may achieve the desired biomimetic characteristics with regard to biocompatibility and biomimicry by adding different synthetic and biological materials to the electrospinning nanofibers. Because tissue composition exhibits gradient features from the top layer that withstands high pressure to the bottom layer that connects with the subchondral bone, gradient scaffolds are needed for cartilage tissue engineering. Fibers generated during electrospinning tend to accumulate in a limited thickness and form a denser instead of thicker scaffold; therefore, strategies of fabricating thicker 3D electrospun scaffolds are crucial.


### 1.3. Objectives

The objective of this paper is to review and discuss the recent trends of electrospinning strategies for cartilage tissue engineering, particularly the biomimetic, gradient, and 3D scaffolds, along with future prospects of potential clinical applications in this field of research.


## 1.1. Electrospinning

An electrospinning system is comprised of at least three units: a high voltage power unit, a material delivery unit (a capillary tube with a small spinneret in general), and a fiber collection unit. A typical electrospinning setup is shown in Figure1 [6]. The randomly distributed nanofibers were collected in Figure 1 on a vertical plate. Usually, an advancement pump is employed to regulate the flow rate of polymeric solution discharged from a syringe. An electrically charged jet of polymer solution or melt is created by a high voltage source. The discharged polymer solution jet goes through an instability process, during which the jet is elongated and the solvent evaporates or solidifies. The jet is finally collected as an interconnected web of ultrathin fibers at the collector that is grounded or connected to an electrode. The diameters of electrospun fibers can range from 10 nm to 100 μm depending on the material, device configuration, and process setup.Figure 1
Typical electrospinning facility with a plate collector [6].Electrospinning is able to generate loosely connected porous mats from submicrometer to nanometer scales in diameter as it is a highly flexible technique to produce continuous fibers. The nanofiber mat yields a high surface area to volume ratio and high porosity [54]. The nanostructure of the mat mimics the structure of the ECM in terms of both morphology and composition [55]. Various patterns of electrospun nanofibers have been fabricated for different biomedical applications ranging from artificial skin to endocrine organs and from the nervous system to cardiovascular tissues [56].


## 1.2. Electrospun Scaffolds for Cartilage Tissue Engineering

Electrospinning as a feasible and versatile technique can manipulate both natural and artificial polymers in nanoscale and promote the proliferation of mesenchymal stem cells (MSCs). Recent research attention has focused on improving the material design of the composition to produce biomimetic, gradient, and 3D scaffolds. Biomimetic scaffold is crucial in the reconstruction of connective tissue such as articular cartilage. Electrospinning may achieve the desired biomimetic characteristics with regard to biocompatibility and biomimicry by adding different synthetic and biological materials to the electrospinning nanofibers. Because tissue composition exhibits gradient features from the top layer that withstands high pressure to the bottom layer that connects with the subchondral bone, gradient scaffolds are needed for cartilage tissue engineering. Fibers generated during electrospinning tend to accumulate in a limited thickness and form a denser instead of thicker scaffold; therefore, strategies of fabricating thicker 3D electrospun scaffolds are crucial.


## 1.3. Objectives

The objective of this paper is to review and discuss the recent trends of electrospinning strategies for cartilage tissue engineering, particularly the biomimetic, gradient, and 3D scaffolds, along with future prospects of potential clinical applications in this field of research.


## 2. Method of Literature Search

Literature selection for this article was based on PubMed, Scopus, Google Scholar, ScienceDirect, and Web of Science databases from 2011 to the present, as the last review paper on this topic was published in 2012 [57]. The search was conducted using different combinations of the following terms: “tissue engineering,” “electrospinning,” “cartilage,” “scaffold,” and “bioscaffold.” Articles that were considered to be related to this review and written in English were included.


## 3. Literature Review

The current literature review reveals that the most prevailing recent trend is the fabrication of biomimetic, gradient, and 3D bioscaffolds, as presented below.


### 3.1. Biomimetic Composite Scaffolds

The desired characteristics of electrospun scaffold for cartilage regeneration include biocompatibility and biomimicry. Different synthetic and biological materials may be added to electrospinning nanofibers to achieve these characteristics. Cao et al. added graphene oxide with poly(vinyl alcohol) (PVA) and chitosan for better biocompatibility and produced uniform nanofibers with improved cell growth rate compared with nanofibers of chitosan and PVA alone [23]. Bioprinting and electrospinning were combined to fabricate biomimetic scaffolds for cartilage tissue engineering [13]. Electrospun fiber assembled hydrogel was also utilized for supplementation of glycosaminoglycan enriched and mineralized cartilage [18].


#### 3.1.1. Structure Biomimicry

Combination of natural and artificial polymers for scaffolds fabrication is considered promising for repair of cartilage defect or damage. For example, better chondrocytes adhesion and spreading efficiency were achieved with a poly(L-lactic-acid) (PLLA)/silk fibroin (SF) composite scaffold [20]. Poly(L-lactide-co-caprolactone) (P(LL-CL)) and gelatin were used for porous scaffolds fabrication to improve water absorption, cell infiltration, and shape-forming [21]. He et al. investigated the feasibility of collagen/poly(L-lactic acid-co-ε-caprolactone) membranes to facilitate cartilage-like tissue formation [14]. Similarly, Sadeghi et al. blended polyhydroxybutyrate (PHB) with chitosan (CTS) to produce hydrophilic fibrous scaffold for better chondrocytes attachment [22]. The advantages of gelatin/polycaprolactone (PCL) on the formation of 3D cartilage regeneration have also been demonstrated [17, 58].Biocompatible polymers can be electrospun with wound healing and antimicrobial agents, such as alkanin and shikonin, to achieve high drug capturing efficiencies and multifunctional activities [11]. Yin et al. fabricated core-shell structure nanofibers with embedded kartogenin solution as core fluid to facilitate cartilage regeneration [24]. Mirzaei et al. incorporated glucosamine into PLLA/PEG scaffolds to achieve an enhanced cell proliferation rate [25]. These composite structures can be used to facilitate chondrogenic differentiation and cartilage repair. Oriented electrospinning scaffold thereby exhibits superb biomimicry of articular cartilage by modifying cell adhesion and distribution.Posttreatment can also benefit biomimetic scaffold fabrication. Liu et al. freeze-dried electrospun fibers with a tricalcium phosphate and produced a trilayered scaffold consisting of oriented fibrous network providing promoted orientation of mesenchymal stem cells [15].


#### 3.1.2. Signal Biomimicry

Sustained and stable release of biomolecules such as growth factors, biological signals, and proteins remains an issue that needs to be resolved. Growth factors such as Nel-like molecule-1 have been preloaded in nanofibers via two-phase electrospinning to achieve prolonged release time as well as enhanced MSCs growth rate [26]. A core-sheath structure fibrous electrospun scaffold was fabricated by Man et al. Using a polyvinyl pyrrolidone/bovine serum albumin/rhTGF-β1 composite solution as the core fluid and poly(ε-caprolactone) solution as the sheath fluid, the scaffolds revealed sustained rhTGF-β1 release and promoted chondrogenic differentiation [16]. MSC chondrogenesis was also enhanced on cellulose derived glycosaminoglycan mimetic scaffolds by Huang et al., given that glycosaminoglycans provide signaling cues in native cartilage tissue [19]. Liao et al. coated cartilaginous ECM on electrospun PCL microfiber scaffolds to enhance MSC chondrogenesis [59]. Composite scaffolds such as poly(vinyl alcohol)/polycaprolactone (PVA/PCL) scaffold seeded with MSC also showed better cartilage defects healing effect [12].Some important electrospinning-based methods to fabricate biomimetic composite scaffolds for cartilage tissue engineering are summarized in Table1. All of the papers cited in Table 1 are directly or possibly related to articular cartilage tissue engineering applications, such as tracheal cartilage engineering.Table 1
Summary of electrospinning-based techniques for fabrication of biomimetic composite scaffolds.
Authors Year Technique Results Application Kontogiannopoulos et al. [11] 2011 Incorporated wound healing and antimicrobial agents High drug entrapment efficiencies and multifunctional activities Tissue engineering scaffolds  Shafiee et al. [12] 2011 Seed MSC in electrospun scaffold Improved cartilage defects healing Bone and cartilage tissue engineering  Xu et al. [13] 2012 Bioprinting and electrospinning 80% survived chondrocytes and cartilage-like tissue formation Cartilage tissue engineering  He et al. [14] 2013 Electrospinning Cartilage-like tissue formation Cartilage tissue engineering  Liu et al. [15] 2014 Freeze-dried electrospinning Successful regenerated osteochondral defects Triphasic osteochondral implant  Man et al. [16] 2014 Electrospinning Sustained rhTGF-β1 release and better chondrogenic differentiation Cartilage tissue engineering  Zheng et al. [17] 2014 Electrospinning 3D cartilage regeneration Cartilage tissue engineering  Mohan et al. [18] 2015 Electrospun fiber assembled hydrogel Sustained release of chondroitin sulfate Cartilage tissue engineering  Huang et al. [19] 2016 Electrospinning Enhanced MSC chondrogenesis Cartilage tissue engineering  Li et al. [20] 2016 Composite electrospinning Better chondrocytes adhesion and filtration Cartilage tissue engineering  Kalaithong et al. [21] 2016 Electrospinning and wet spinning Better water absorption and cell infiltration Cartilage tissue engineering  Sadeghi et al. [22] 2016 Electrospinning Better hydrophilic property and cell attachment Cartilage tissue engineering  Cao et al. [23] 2017 Chitosan/graphene oxide polymer nanofiber Better biocompatibility and cell growth rate Cartilage tissue engineering  Yin et al. [24] 2017 Core-shell structure nanofiber with embedded kartogenin solution Promoted chondrogenic differentiation Tracheal cartilage regeneration  Mirzaei et al. [25] 2017 Glucosamine incorporated into PLLA/PEG scaffolds Enhanced cell proliferation rate Cartilage tissue engineering  Wang et al. [26] 2017 Two-phase electrospinning Prolonged drug release time and enhanced MSCs growth rate Cartilage tissue engineering


### 3.2. Gradient Scaffolds

Several methods of generating gradient scaffolds have been reported by researchers such as structure and composition gradient. He et al. first deposited a layer of aligned nanofibers of pure poly(L-lactide-co-glycolide) acid (PLGA) on a cylindrical surface and then deposited a layer of aligned nanofibers of PLGA/nanohydroxyapatite (HA) on top. The microstructural organization and nano-HA content in electrospun scaffolds exhibit gradient change [33] and the anisotropic strain was also eliminated in scaffolds with fiber diameter gradient in Grey et al.’s research [30]. Guided spatial differentiation of MSCs [28] was also observed in composition and biomolecule gradient scaffolds. The scaffolds exhibit superior material properties in burst testing. The biodegradation rate and biological functions were controlled in Angarano et al.’s fiber diameter gradient scaffolds [31].Fabricating scaffolds with gradients of molecules and element particles for tissue engineering has drawn substantial attention. Chondroitin sulfate (CS) and gentamycin sulfate (GS) gradients have been achieved with mineralized cartilage [18] and spatiotemporal drug release [35]. Ramalingam et al. reported a scaffold with amorphous calcium phosphate nanoparticles (nACP) gradient by coelectrospinning. Adhesion and proliferation of osteogenic cells were enhanced in gradient regions that have higher nACP concentration with a graded osteoblast response [29]. The graded cells’ outgrowth rate and osteogenesis were also found to be positively related to the protein concentration gradient [27] and mineral gradient [34] on scaffolds, respectively.Scaffolds with chemical and mechanical property gradient have also been investigated. Samavedi et al. demonstrated the possibility of fabricating a mechanochemical gradient scaffold with graded meshes by using controlled infusion of encapsulated CaCO3 and TiO2 nanoparticles [60]. The cell viability has shown preliminary evidence regarding the suitability of these scaffolds forin vitro tissue engineering.Some important electrospinning-based methods to fabricate gradient scaffolds used in cartilage tissue engineering are summarized in Table2. All of the papers cited in Table 2 are directly or possibly related to articular cartilage tissue engineering applications, such as interfacial tissue engineering and soft tissue regeneration.Table 2
Summary of electrospinning-based techniques for fabricating gradient scaffolds.
Authors Year Gradient parameter(s) Technique Results Application Zander et al. [27] 2012 Protein concentration gradient Air-plasma-modified electrospinning Corresponding cell outgrowth rate Tissue engineering  Zhang et al. [28] 2012 Composition and biomolecule gradient Microfluidic assisted electrospinning Guided spatial cell differentiation Tissue engineering  Ramalingam et al. [29] 2013 Composition gradient Coelectrospinning Enhanced osteogenic cells proliferation and adhesion Interfacial tissue engineering  Grey et al. [30] 2013 Fiber diameter gradient Gradient electrospinning Enhanced mechanical properties Tissue engineering  Angarano et al. [31] 2013 Fiber diameter gradient Reactive electrospinning Gradient biodegradation rate Soft tissue regeneration  Sundararaghavan et al. [32] 2013 Growth factor gradient Gradient electrospinning Directed cell motility in gradient direction Tissue engineering  He et al. [33] 2014 Structure and composition gradient Modified coelectrospinning Gradient cell metabolic activity Tissue engineering  Liu et al. [34] 2014 Mineral gradient Graded mineral coating Graded mesenchymal stem cells osteogenesis Interfacial tissue engineering  Mohan et al. [18] 2015 CS and BG gradient Electrospun fiber assembled hydrogel Glycosaminoglycan enriched and mineralized cartilage formation Cartilage tissue engineering  Liu et al. [35] 2016 GS and deferoxamine 3D bioprinting and electrospinning Spatiotemporal drug release Osteochondral tissue engineering


### 3.3. 2D Scaffolds versus 3D Scaffolds

One of the major issues of conventional electrospun nanofibrous scaffolds is the limited thickness (typically < 1 mm) [61]. While 2D scaffolds are widely used in tissue engineering applications, they still fall short of contributing to crucial factors such as cell communication in ECM context, mechanical cues, and nutrient transportation [62]. 3D scaffolds, on the other hand, have superior cell differentiation and development rate, especially for connective tissues such as articular cartilage [53], and can improve cell infiltration rate with larger pore size and higher porosity [50]. The oriented electrospun fibers in 3D scale can guide the MSCs to grow in certain direction and further promote the formation of oriented and connective tissue. Further, in fabricating 3D multiphasic scaffolds where the scaffolds are separated spatially into different sections for guided MSCs differentiation mimicking the structure of connective tissues such as articular cartilage, electrospinning as a less complicated process for producing aligned fibers in 3D scale could demonstrate advantages in fabricating multiphasic scaffolds.Among a multitude of applications for 3D organization of the nanofibers, processing the nanofibrous mesh into a desirable form after electrospinning has attracted substantial interest. For example, a 3D scaffold can be created by stacking multiple layers of nanofiber mesh for cell seeding [48]. Garrigues et al. found that multilayer scaffolds enhanced cell infiltration aggrecan (ACAN) gene expression [46]. Yunos et al. designed a bilayered scaffold by combining electrospun fibers with bioglass and obtained viable chondrocyte cells in the scaffold [43]. Xue et al. prepared the electrospun gelatin/PCL membranes into rounded shape with seeded chondrocytes to culture an ear-shaped cartilage, with good elasticity and impressive mechanical strength [45]. Kai et al. incorporated electrospun fibers into hydrogel to improve mechanical properties such as compressive strength [39]. The advantage of this simple method is the high degree of flexibility in creating the ultimate geometry of scaffolds.Modified electrospinning setups can also be utilized for 3D structure such as electrospinning with external heat source [38] and dual nozzle extrusion system to improve cell infiltration rate. He et al. increased the pore size of scaffolds by near-field electrospinning [63]. Levorson et al. also increased cellular infiltration with multiscale scaffold, which contains microfibers and nanofibers evenly distributed throughout the entire construct [44]. Human mesenchymal cells were found to maintain scaffold cellularity under serum-free conditions with these scaffolds. A fluffy 3D scaffold with randomly and evenly oriented fibers in all directions was also fabricated by utilizing the electrostatic repulsion between fibers; the cell proliferation rate observed was 5 times as fast as the 2D scaffold counterparts after one week [42].Novel electrospinning solutions have also been investigated for 3D electrospinning. For example, Xu et al. started from a polymer solution with de-cross-linked keratin from chicken feathers to obtain intrinsic water stability for 3D scaffold [47]. Enhancement of cartilage repairing can also be achieved by scaffolds with cross-linked hyaluronic acid [51] and biological cue chondroitin sulfate-incorporated electrospinning [37]. Wei et al. combined poly[(butylene succinate)-co-adipate] (PBSA) and PLLA to culture primary human chondrocytes (PHCs) in electrospun 3D fibrous scaffolds for improved cell attachment and proliferation [40].Another strategy for fabricating 3D scaffold is combining electrospinning with other advanced manufacturing techniques such as 3D printing and freeze-drying. In the research by Xu et al. about hybrid inkjet printing and electrospinning system, the cell viability was 80% after one week, and cartilage-like tissue has formed bothin vitro andin vivo [13]. Afonso et al. combined another advanced manufacturing technique, direct writing, with electrospinning to obtain oriented fibers and a highly controlled scaffold structure [52]. Liu et al. enhanced the mechanical strength of electrospinning by freeze-drying, and osteochondral defects were repaired in a rabbit model [49].Last but not least, 3D structure can be achieved with different postprocess treatments. Holmes et al. improved mechanical properties of the 3D scaffolds with hydrogen treated multiwalled carbon nanotubes (MWCNTs) [41]. Zhu et al.’s scaffolds enhanced chondrogenic differentiation and cell infiltration rate with cold atmospheric plasma treated electrospinning [50]. Chen and Su also demonstrated better viability, proliferation, and differentiation of rabbit articular chondrocytes, with plasma-treatment electrospun scaffold [36].Some important electrospinning-based methods to construct 3D nanostructures for the scaffolds used in tissue engineering are summarized in Table3. All of the papers cited in Table 3 are directly or possibly related to articular cartilage tissue engineering applications, such as osteochondral tissue replacement and MSC chondrogenesis.Table 3
Summary of electrospinning-based techniques for fabricating 3D nanofibrous structure.
Authors Year Technique Advantage(s) Disadvantage(s) Application Chen and Su [36] 2011 Electrospinning with plasma treatment Enhanced chondrocytes viability and proliferation N/A Cartilage tissue engineering  Coburn et al. [37] 2012 Biological cue chondroitin sulfate incorporated electrospinning Enhanced cartilaginous formation Weak mechanical properties Cartilage tissue engineering  Shabani et al. [38] 2012 Modified setup of electrospinning with heat from halogen light bulbs Improved cell infiltration rate Material limitation Tissue engineering  Kai et al. [39] 2012 Nanofiber with hydrogel Relatively higher compressive strength No significant cell proliferation improvement Tissue regeneration  Xu et al. [13] 2012 Hybrid inkjet printing/electrospinning system High cell viability, formed cartilage-like structure Further refinement required Cartilage tissue engineering  Wei et al. [40] 2012 Electrospinning Improved cell attachment and proliferation N/A Cartilage tissue engineering  Holmes et al. [41] 2013 Hydrogen treated multiwalled carbon nanotubes (MWCNTs) Higher mechanical strength and cell differentiation Unclear effect of MWCNTsin vivo MSC chondrogenesis  Cai et al. [42] 2013 Electrostatic repulsion Randomly and evenly oriented 3D fibers Rapid delivery of electrons on fibers required Cell culture for soft tissues  Yunos et al. [43] 2013 Bilayered scaffold Chondrocyte cell-supporting ability Decreased HA formation rate with thicker layer Osteochondral tissue replacement  Levorson et al. [44] 2013 Dual extrusion electrospinning Maintained scaffold cellularity Lack of parameter optimization Cartilage tissue engineering  Xue et al. [45] 2014 Prepare the electrospun membrane in rounded shape Formed ear-shaped cartilage tissue Lack of immunogenicity investigation Cartilage tissue engineering  Garrigues et al. [46] 2014 Electrospinning Enhanced cell infiltration Lower elastic modulus Cartilage tissue engineering  Xu et al. [47] 2014 Electrospinning solution with de-cross-linked keratin from chicken feathers Intrinsic water stability Randomly oriented fibers Cell penetration and differentiation  Orr et al. [48] 2015 Vertical stacking layers of fiber membrane Easy to seed cells on surface prior to stacking Cells unable to penetrate through layers Compressive loading applications  Liu et al. [49] 2015 Electrospinning and freeze drying Better mechanical strength N/A Cartilage tissue engineering  Zhu et al. [50] 2015 Electrospinning with cold atmospheric plasma treatment Enhanced chondrogenic differentiation and cell infiltration Small thickness for 3D scaffold Cartilage tissue engineering  Chen et al. [51] 2016 Modified scaffold with cross-linked hyaluronic acid Superabsorbent property and excellent cytocompatibility Complicated fabrication process Cartilage tissue engineering  Afonso et al. [52] 2016 Direct writing electrospinning Directed tissue organization and fibril matrix orientation Microscale fibers Tissue engineering  Damaraju et al. [53] 2017 Piezoelectric fibrous scaffolds Promoted mesenchymal stem cell differentiation N/A Cartilage and bone tissue engineering


## 3.1. Biomimetic Composite Scaffolds

The desired characteristics of electrospun scaffold for cartilage regeneration include biocompatibility and biomimicry. Different synthetic and biological materials may be added to electrospinning nanofibers to achieve these characteristics. Cao et al. added graphene oxide with poly(vinyl alcohol) (PVA) and chitosan for better biocompatibility and produced uniform nanofibers with improved cell growth rate compared with nanofibers of chitosan and PVA alone [23]. Bioprinting and electrospinning were combined to fabricate biomimetic scaffolds for cartilage tissue engineering [13]. Electrospun fiber assembled hydrogel was also utilized for supplementation of glycosaminoglycan enriched and mineralized cartilage [18].


### 3.1.1. Structure Biomimicry

Combination of natural and artificial polymers for scaffolds fabrication is considered promising for repair of cartilage defect or damage. For example, better chondrocytes adhesion and spreading efficiency were achieved with a poly(L-lactic-acid) (PLLA)/silk fibroin (SF) composite scaffold [20]. Poly(L-lactide-co-caprolactone) (P(LL-CL)) and gelatin were used for porous scaffolds fabrication to improve water absorption, cell infiltration, and shape-forming [21]. He et al. investigated the feasibility of collagen/poly(L-lactic acid-co-ε-caprolactone) membranes to facilitate cartilage-like tissue formation [14]. Similarly, Sadeghi et al. blended polyhydroxybutyrate (PHB) with chitosan (CTS) to produce hydrophilic fibrous scaffold for better chondrocytes attachment [22]. The advantages of gelatin/polycaprolactone (PCL) on the formation of 3D cartilage regeneration have also been demonstrated [17, 58].Biocompatible polymers can be electrospun with wound healing and antimicrobial agents, such as alkanin and shikonin, to achieve high drug capturing efficiencies and multifunctional activities [11]. Yin et al. fabricated core-shell structure nanofibers with embedded kartogenin solution as core fluid to facilitate cartilage regeneration [24]. Mirzaei et al. incorporated glucosamine into PLLA/PEG scaffolds to achieve an enhanced cell proliferation rate [25]. These composite structures can be used to facilitate chondrogenic differentiation and cartilage repair. Oriented electrospinning scaffold thereby exhibits superb biomimicry of articular cartilage by modifying cell adhesion and distribution.Posttreatment can also benefit biomimetic scaffold fabrication. Liu et al. freeze-dried electrospun fibers with a tricalcium phosphate and produced a trilayered scaffold consisting of oriented fibrous network providing promoted orientation of mesenchymal stem cells [15].


### 3.1.2. Signal Biomimicry

Sustained and stable release of biomolecules such as growth factors, biological signals, and proteins remains an issue that needs to be resolved. Growth factors such as Nel-like molecule-1 have been preloaded in nanofibers via two-phase electrospinning to achieve prolonged release time as well as enhanced MSCs growth rate [26]. A core-sheath structure fibrous electrospun scaffold was fabricated by Man et al. Using a polyvinyl pyrrolidone/bovine serum albumin/rhTGF-β1 composite solution as the core fluid and poly(ε-caprolactone) solution as the sheath fluid, the scaffolds revealed sustained rhTGF-β1 release and promoted chondrogenic differentiation [16]. MSC chondrogenesis was also enhanced on cellulose derived glycosaminoglycan mimetic scaffolds by Huang et al., given that glycosaminoglycans provide signaling cues in native cartilage tissue [19]. Liao et al. coated cartilaginous ECM on electrospun PCL microfiber scaffolds to enhance MSC chondrogenesis [59]. Composite scaffolds such as poly(vinyl alcohol)/polycaprolactone (PVA/PCL) scaffold seeded with MSC also showed better cartilage defects healing effect [12].Some important electrospinning-based methods to fabricate biomimetic composite scaffolds for cartilage tissue engineering are summarized in Table1. All of the papers cited in Table 1 are directly or possibly related to articular cartilage tissue engineering applications, such as tracheal cartilage engineering.Table 1
Summary of electrospinning-based techniques for fabrication of biomimetic composite scaffolds.
Authors Year Technique Results Application Kontogiannopoulos et al. [11] 2011 Incorporated wound healing and antimicrobial agents High drug entrapment efficiencies and multifunctional activities Tissue engineering scaffolds  Shafiee et al. [12] 2011 Seed MSC in electrospun scaffold Improved cartilage defects healing Bone and cartilage tissue engineering  Xu et al. [13] 2012 Bioprinting and electrospinning 80% survived chondrocytes and cartilage-like tissue formation Cartilage tissue engineering  He et al. [14] 2013 Electrospinning Cartilage-like tissue formation Cartilage tissue engineering  Liu et al. [15] 2014 Freeze-dried electrospinning Successful regenerated osteochondral defects Triphasic osteochondral implant  Man et al. [16] 2014 Electrospinning Sustained rhTGF-β1 release and better chondrogenic differentiation Cartilage tissue engineering  Zheng et al. [17] 2014 Electrospinning 3D cartilage regeneration Cartilage tissue engineering  Mohan et al. [18] 2015 Electrospun fiber assembled hydrogel Sustained release of chondroitin sulfate Cartilage tissue engineering  Huang et al. [19] 2016 Electrospinning Enhanced MSC chondrogenesis Cartilage tissue engineering  Li et al. [20] 2016 Composite electrospinning Better chondrocytes adhesion and filtration Cartilage tissue engineering  Kalaithong et al. [21] 2016 Electrospinning and wet spinning Better water absorption and cell infiltration Cartilage tissue engineering  Sadeghi et al. [22] 2016 Electrospinning Better hydrophilic property and cell attachment Cartilage tissue engineering  Cao et al. [23] 2017 Chitosan/graphene oxide polymer nanofiber Better biocompatibility and cell growth rate Cartilage tissue engineering  Yin et al. [24] 2017 Core-shell structure nanofiber with embedded kartogenin solution Promoted chondrogenic differentiation Tracheal cartilage regeneration  Mirzaei et al. [25] 2017 Glucosamine incorporated into PLLA/PEG scaffolds Enhanced cell proliferation rate Cartilage tissue engineering  Wang et al. [26] 2017 Two-phase electrospinning Prolonged drug release time and enhanced MSCs growth rate Cartilage tissue engineering


## 3.1.1. Structure Biomimicry

Combination of natural and artificial polymers for scaffolds fabrication is considered promising for repair of cartilage defect or damage. For example, better chondrocytes adhesion and spreading efficiency were achieved with a poly(L-lactic-acid) (PLLA)/silk fibroin (SF) composite scaffold [20]. Poly(L-lactide-co-caprolactone) (P(LL-CL)) and gelatin were used for porous scaffolds fabrication to improve water absorption, cell infiltration, and shape-forming [21]. He et al. investigated the feasibility of collagen/poly(L-lactic acid-co-ε-caprolactone) membranes to facilitate cartilage-like tissue formation [14]. Similarly, Sadeghi et al. blended polyhydroxybutyrate (PHB) with chitosan (CTS) to produce hydrophilic fibrous scaffold for better chondrocytes attachment [22]. The advantages of gelatin/polycaprolactone (PCL) on the formation of 3D cartilage regeneration have also been demonstrated [17, 58].Biocompatible polymers can be electrospun with wound healing and antimicrobial agents, such as alkanin and shikonin, to achieve high drug capturing efficiencies and multifunctional activities [11]. Yin et al. fabricated core-shell structure nanofibers with embedded kartogenin solution as core fluid to facilitate cartilage regeneration [24]. Mirzaei et al. incorporated glucosamine into PLLA/PEG scaffolds to achieve an enhanced cell proliferation rate [25]. These composite structures can be used to facilitate chondrogenic differentiation and cartilage repair. Oriented electrospinning scaffold thereby exhibits superb biomimicry of articular cartilage by modifying cell adhesion and distribution.Posttreatment can also benefit biomimetic scaffold fabrication. Liu et al. freeze-dried electrospun fibers with a tricalcium phosphate and produced a trilayered scaffold consisting of oriented fibrous network providing promoted orientation of mesenchymal stem cells [15].


## 3.1.2. Signal Biomimicry

Sustained and stable release of biomolecules such as growth factors, biological signals, and proteins remains an issue that needs to be resolved. Growth factors such as Nel-like molecule-1 have been preloaded in nanofibers via two-phase electrospinning to achieve prolonged release time as well as enhanced MSCs growth rate [26]. A core-sheath structure fibrous electrospun scaffold was fabricated by Man et al. Using a polyvinyl pyrrolidone/bovine serum albumin/rhTGF-β1 composite solution as the core fluid and poly(ε-caprolactone) solution as the sheath fluid, the scaffolds revealed sustained rhTGF-β1 release and promoted chondrogenic differentiation [16]. MSC chondrogenesis was also enhanced on cellulose derived glycosaminoglycan mimetic scaffolds by Huang et al., given that glycosaminoglycans provide signaling cues in native cartilage tissue [19]. Liao et al. coated cartilaginous ECM on electrospun PCL microfiber scaffolds to enhance MSC chondrogenesis [59]. Composite scaffolds such as poly(vinyl alcohol)/polycaprolactone (PVA/PCL) scaffold seeded with MSC also showed better cartilage defects healing effect [12].Some important electrospinning-based methods to fabricate biomimetic composite scaffolds for cartilage tissue engineering are summarized in Table1. All of the papers cited in Table 1 are directly or possibly related to articular cartilage tissue engineering applications, such as tracheal cartilage engineering.Table 1
Summary of electrospinning-based techniques for fabrication of biomimetic composite scaffolds.
Authors Year Technique Results Application Kontogiannopoulos et al. [11] 2011 Incorporated wound healing and antimicrobial agents High drug entrapment efficiencies and multifunctional activities Tissue engineering scaffolds  Shafiee et al. [12] 2011 Seed MSC in electrospun scaffold Improved cartilage defects healing Bone and cartilage tissue engineering  Xu et al. [13] 2012 Bioprinting and electrospinning 80% survived chondrocytes and cartilage-like tissue formation Cartilage tissue engineering  He et al. [14] 2013 Electrospinning Cartilage-like tissue formation Cartilage tissue engineering  Liu et al. [15] 2014 Freeze-dried electrospinning Successful regenerated osteochondral defects Triphasic osteochondral implant  Man et al. [16] 2014 Electrospinning Sustained rhTGF-β1 release and better chondrogenic differentiation Cartilage tissue engineering  Zheng et al. [17] 2014 Electrospinning 3D cartilage regeneration Cartilage tissue engineering  Mohan et al. [18] 2015 Electrospun fiber assembled hydrogel Sustained release of chondroitin sulfate Cartilage tissue engineering  Huang et al. [19] 2016 Electrospinning Enhanced MSC chondrogenesis Cartilage tissue engineering  Li et al. [20] 2016 Composite electrospinning Better chondrocytes adhesion and filtration Cartilage tissue engineering  Kalaithong et al. [21] 2016 Electrospinning and wet spinning Better water absorption and cell infiltration Cartilage tissue engineering  Sadeghi et al. [22] 2016 Electrospinning Better hydrophilic property and cell attachment Cartilage tissue engineering  Cao et al. [23] 2017 Chitosan/graphene oxide polymer nanofiber Better biocompatibility and cell growth rate Cartilage tissue engineering  Yin et al. [24] 2017 Core-shell structure nanofiber with embedded kartogenin solution Promoted chondrogenic differentiation Tracheal cartilage regeneration  Mirzaei et al. [25] 2017 Glucosamine incorporated into PLLA/PEG scaffolds Enhanced cell proliferation rate Cartilage tissue engineering  Wang et al. [26] 2017 Two-phase electrospinning Prolonged drug release time and enhanced MSCs growth rate Cartilage tissue engineering


## 3.2. Gradient Scaffolds

Several methods of generating gradient scaffolds have been reported by researchers such as structure and composition gradient. He et al. first deposited a layer of aligned nanofibers of pure poly(L-lactide-co-glycolide) acid (PLGA) on a cylindrical surface and then deposited a layer of aligned nanofibers of PLGA/nanohydroxyapatite (HA) on top. The microstructural organization and nano-HA content in electrospun scaffolds exhibit gradient change [33] and the anisotropic strain was also eliminated in scaffolds with fiber diameter gradient in Grey et al.’s research [30]. Guided spatial differentiation of MSCs [28] was also observed in composition and biomolecule gradient scaffolds. The scaffolds exhibit superior material properties in burst testing. The biodegradation rate and biological functions were controlled in Angarano et al.’s fiber diameter gradient scaffolds [31].Fabricating scaffolds with gradients of molecules and element particles for tissue engineering has drawn substantial attention. Chondroitin sulfate (CS) and gentamycin sulfate (GS) gradients have been achieved with mineralized cartilage [18] and spatiotemporal drug release [35]. Ramalingam et al. reported a scaffold with amorphous calcium phosphate nanoparticles (nACP) gradient by coelectrospinning. Adhesion and proliferation of osteogenic cells were enhanced in gradient regions that have higher nACP concentration with a graded osteoblast response [29]. The graded cells’ outgrowth rate and osteogenesis were also found to be positively related to the protein concentration gradient [27] and mineral gradient [34] on scaffolds, respectively.Scaffolds with chemical and mechanical property gradient have also been investigated. Samavedi et al. demonstrated the possibility of fabricating a mechanochemical gradient scaffold with graded meshes by using controlled infusion of encapsulated CaCO3 and TiO2 nanoparticles [60]. The cell viability has shown preliminary evidence regarding the suitability of these scaffolds forin vitro tissue engineering.Some important electrospinning-based methods to fabricate gradient scaffolds used in cartilage tissue engineering are summarized in Table2. All of the papers cited in Table 2 are directly or possibly related to articular cartilage tissue engineering applications, such as interfacial tissue engineering and soft tissue regeneration.Table 2
Summary of electrospinning-based techniques for fabricating gradient scaffolds.
Authors Year Gradient parameter(s) Technique Results Application Zander et al. [27] 2012 Protein concentration gradient Air-plasma-modified electrospinning Corresponding cell outgrowth rate Tissue engineering  Zhang et al. [28] 2012 Composition and biomolecule gradient Microfluidic assisted electrospinning Guided spatial cell differentiation Tissue engineering  Ramalingam et al. [29] 2013 Composition gradient Coelectrospinning Enhanced osteogenic cells proliferation and adhesion Interfacial tissue engineering  Grey et al. [30] 2013 Fiber diameter gradient Gradient electrospinning Enhanced mechanical properties Tissue engineering  Angarano et al. [31] 2013 Fiber diameter gradient Reactive electrospinning Gradient biodegradation rate Soft tissue regeneration  Sundararaghavan et al. [32] 2013 Growth factor gradient Gradient electrospinning Directed cell motility in gradient direction Tissue engineering  He et al. [33] 2014 Structure and composition gradient Modified coelectrospinning Gradient cell metabolic activity Tissue engineering  Liu et al. [34] 2014 Mineral gradient Graded mineral coating Graded mesenchymal stem cells osteogenesis Interfacial tissue engineering  Mohan et al. [18] 2015 CS and BG gradient Electrospun fiber assembled hydrogel Glycosaminoglycan enriched and mineralized cartilage formation Cartilage tissue engineering  Liu et al. [35] 2016 GS and deferoxamine 3D bioprinting and electrospinning Spatiotemporal drug release Osteochondral tissue engineering


## 3.3. 2D Scaffolds versus 3D Scaffolds

One of the major issues of conventional electrospun nanofibrous scaffolds is the limited thickness (typically < 1 mm) [61]. While 2D scaffolds are widely used in tissue engineering applications, they still fall short of contributing to crucial factors such as cell communication in ECM context, mechanical cues, and nutrient transportation [62]. 3D scaffolds, on the other hand, have superior cell differentiation and development rate, especially for connective tissues such as articular cartilage [53], and can improve cell infiltration rate with larger pore size and higher porosity [50]. The oriented electrospun fibers in 3D scale can guide the MSCs to grow in certain direction and further promote the formation of oriented and connective tissue. Further, in fabricating 3D multiphasic scaffolds where the scaffolds are separated spatially into different sections for guided MSCs differentiation mimicking the structure of connective tissues such as articular cartilage, electrospinning as a less complicated process for producing aligned fibers in 3D scale could demonstrate advantages in fabricating multiphasic scaffolds.Among a multitude of applications for 3D organization of the nanofibers, processing the nanofibrous mesh into a desirable form after electrospinning has attracted substantial interest. For example, a 3D scaffold can be created by stacking multiple layers of nanofiber mesh for cell seeding [48]. Garrigues et al. found that multilayer scaffolds enhanced cell infiltration aggrecan (ACAN) gene expression [46]. Yunos et al. designed a bilayered scaffold by combining electrospun fibers with bioglass and obtained viable chondrocyte cells in the scaffold [43]. Xue et al. prepared the electrospun gelatin/PCL membranes into rounded shape with seeded chondrocytes to culture an ear-shaped cartilage, with good elasticity and impressive mechanical strength [45]. Kai et al. incorporated electrospun fibers into hydrogel to improve mechanical properties such as compressive strength [39]. The advantage of this simple method is the high degree of flexibility in creating the ultimate geometry of scaffolds.Modified electrospinning setups can also be utilized for 3D structure such as electrospinning with external heat source [38] and dual nozzle extrusion system to improve cell infiltration rate. He et al. increased the pore size of scaffolds by near-field electrospinning [63]. Levorson et al. also increased cellular infiltration with multiscale scaffold, which contains microfibers and nanofibers evenly distributed throughout the entire construct [44]. Human mesenchymal cells were found to maintain scaffold cellularity under serum-free conditions with these scaffolds. A fluffy 3D scaffold with randomly and evenly oriented fibers in all directions was also fabricated by utilizing the electrostatic repulsion between fibers; the cell proliferation rate observed was 5 times as fast as the 2D scaffold counterparts after one week [42].Novel electrospinning solutions have also been investigated for 3D electrospinning. For example, Xu et al. started from a polymer solution with de-cross-linked keratin from chicken feathers to obtain intrinsic water stability for 3D scaffold [47]. Enhancement of cartilage repairing can also be achieved by scaffolds with cross-linked hyaluronic acid [51] and biological cue chondroitin sulfate-incorporated electrospinning [37]. Wei et al. combined poly[(butylene succinate)-co-adipate] (PBSA) and PLLA to culture primary human chondrocytes (PHCs) in electrospun 3D fibrous scaffolds for improved cell attachment and proliferation [40].Another strategy for fabricating 3D scaffold is combining electrospinning with other advanced manufacturing techniques such as 3D printing and freeze-drying. In the research by Xu et al. about hybrid inkjet printing and electrospinning system, the cell viability was 80% after one week, and cartilage-like tissue has formed bothin vitro andin vivo [13]. Afonso et al. combined another advanced manufacturing technique, direct writing, with electrospinning to obtain oriented fibers and a highly controlled scaffold structure [52]. Liu et al. enhanced the mechanical strength of electrospinning by freeze-drying, and osteochondral defects were repaired in a rabbit model [49].Last but not least, 3D structure can be achieved with different postprocess treatments. Holmes et al. improved mechanical properties of the 3D scaffolds with hydrogen treated multiwalled carbon nanotubes (MWCNTs) [41]. Zhu et al.’s scaffolds enhanced chondrogenic differentiation and cell infiltration rate with cold atmospheric plasma treated electrospinning [50]. Chen and Su also demonstrated better viability, proliferation, and differentiation of rabbit articular chondrocytes, with plasma-treatment electrospun scaffold [36].Some important electrospinning-based methods to construct 3D nanostructures for the scaffolds used in tissue engineering are summarized in Table3. All of the papers cited in Table 3 are directly or possibly related to articular cartilage tissue engineering applications, such as osteochondral tissue replacement and MSC chondrogenesis.Table 3
Summary of electrospinning-based techniques for fabricating 3D nanofibrous structure.
Authors Year Technique Advantage(s) Disadvantage(s) Application Chen and Su [36] 2011 Electrospinning with plasma treatment Enhanced chondrocytes viability and proliferation N/A Cartilage tissue engineering  Coburn et al. [37] 2012 Biological cue chondroitin sulfate incorporated electrospinning Enhanced cartilaginous formation Weak mechanical properties Cartilage tissue engineering  Shabani et al. [38] 2012 Modified setup of electrospinning with heat from halogen light bulbs Improved cell infiltration rate Material limitation Tissue engineering  Kai et al. [39] 2012 Nanofiber with hydrogel Relatively higher compressive strength No significant cell proliferation improvement Tissue regeneration  Xu et al. [13] 2012 Hybrid inkjet printing/electrospinning system High cell viability, formed cartilage-like structure Further refinement required Cartilage tissue engineering  Wei et al. [40] 2012 Electrospinning Improved cell attachment and proliferation N/A Cartilage tissue engineering  Holmes et al. [41] 2013 Hydrogen treated multiwalled carbon nanotubes (MWCNTs) Higher mechanical strength and cell differentiation Unclear effect of MWCNTsin vivo MSC chondrogenesis  Cai et al. [42] 2013 Electrostatic repulsion Randomly and evenly oriented 3D fibers Rapid delivery of electrons on fibers required Cell culture for soft tissues  Yunos et al. [43] 2013 Bilayered scaffold Chondrocyte cell-supporting ability Decreased HA formation rate with thicker layer Osteochondral tissue replacement  Levorson et al. [44] 2013 Dual extrusion electrospinning Maintained scaffold cellularity Lack of parameter optimization Cartilage tissue engineering  Xue et al. [45] 2014 Prepare the electrospun membrane in rounded shape Formed ear-shaped cartilage tissue Lack of immunogenicity investigation Cartilage tissue engineering  Garrigues et al. [46] 2014 Electrospinning Enhanced cell infiltration Lower elastic modulus Cartilage tissue engineering  Xu et al. [47] 2014 Electrospinning solution with de-cross-linked keratin from chicken feathers Intrinsic water stability Randomly oriented fibers Cell penetration and differentiation  Orr et al. [48] 2015 Vertical stacking layers of fiber membrane Easy to seed cells on surface prior to stacking Cells unable to penetrate through layers Compressive loading applications  Liu et al. [49] 2015 Electrospinning and freeze drying Better mechanical strength N/A Cartilage tissue engineering  Zhu et al. [50] 2015 Electrospinning with cold atmospheric plasma treatment Enhanced chondrogenic differentiation and cell infiltration Small thickness for 3D scaffold Cartilage tissue engineering  Chen et al. [51] 2016 Modified scaffold with cross-linked hyaluronic acid Superabsorbent property and excellent cytocompatibility Complicated fabrication process Cartilage tissue engineering  Afonso et al. [52] 2016 Direct writing electrospinning Directed tissue organization and fibril matrix orientation Microscale fibers Tissue engineering  Damaraju et al. [53] 2017 Piezoelectric fibrous scaffolds Promoted mesenchymal stem cell differentiation N/A Cartilage and bone tissue engineering


## 4. Discussion

Electrospinning provides an efficient way of fabricating cartilage tissue engineering scaffolds with nanoscale elements and utilization of a wide range of polymers. The process can be easily modified for various biomedical applications. Although there have been progress and improvements in recent years, very limited research has been reported on complete articular cartilage repair or major improvement in tissue engineering for comprehensive treatment of related diseases such as arthritis. There is hardly any parameter optimization for refined fiber strength and geometry. The complexity of electrospinning setups is growing rapidly as it incorporates more and more novel techniques such as biological cue-incorporated electrospinning [37], hydrogel [39], hybrid 3D printing [13], and cold atmospheric plasma treatment [50]. On one hand, it is highly challenging to deal with greater magnitude of parameters and characteristic architectures. On the other hand, these 3D scaffold strategies incorporating different techniques all come with certain weaknesses or vulnerabilities such as small thickness and microscale (instead of nanoscale) fibers (>200 nm). Therefore, the possibility of clinical application of these techniques on a large scale is still fairly slim.Several electrospinning strategies have been developed for fabricating biomimetic composite scaffolds. Along with antimicrobial agents and growth factors, both structure and signal biomimetic scaffolds produced exhibit suitable biocompatibility and intermediate level of biomimicry. However, the effects of fiber-guided cell orientation on chondrogenic differentiation, attachment, and mineralization of marrow mesenchymal stem cells need to be further investigated and so should optimization for cell culture and electrospinning process.Various improvements in mechanical properties of scaffolds, such as microstructural organization [33], tensile strength [60, 64], and anisotropic strain [30], have been achieved with different gradient properties. However, all of the improved mechanical properties, such as tensile strength, are still in the undesired low range (<10 MPa) [13]. And there are no quantitative results for the effect of enhanced mechanical properties on cell proliferation rate. In some cases, the overall mechanical strength was found to be even lower than that of the control scaffolds with no gradient. To address this issue, 3D electrospun fibers were immersed into a medium, such as hydrogel, to improve their mechanical strengths [39]; however, the electrospun fibers dissolve much faster than hydrogel in cell culture. Also, hardly any research has addressed the issue of mechanical properties of 3D scaffolds. These issues need to have experimental justification to verify that the improvement of these mechanical properties is helpful forin vitroandin vivo cell proliferation.Using different gradient scaffolds, researchers were able to create graded cell response [29], outgrowth rate [27], and biodegradation rate [31] in a single scaffold.In vivo studies are needed to investigate the effects and suitability of these gradient scaffolds employed in cartilage implants, as well as related interfacial tissue engineering.Although electrospun scaffolds possess higher porosity than other forms of scaffolds, a common drawback is the limited size of pores, which further prevents cells from growing in the scaffold [65]. Several measures have been investigated to address this issue, such as using sacrificial fibers [66], multiscale scaffold [44], hybrid scaffold [67], near-field electrospinning [63], and salt leaching and ice crystals [20]. These techniques could also be incorporated in 3D scaffolds fabrication for better cell infiltration.The positive effects of 3D scaffolds on cell infiltration rate [44, 63] and cell proliferation rate [42] have been extensively investigated and verified. Other crucial properties in cell culture such as water stability [47] and cartilage-like tissue formation [37, 51] have also been investigated, demonstrating the intrinsic advantages of 3D scaffolds over 2D scaffolds. The biodegradation rate and biomimicry level should be further characterized quantitatively before 3D scaffolds can be implemented as cartilage implantsin vivo.Electrospun scaffolds for cartilage tissue engineering still face major challenges in biomechanical and biological properties. More novel synthetic and artificial materials need to be explored and tested with regard to issues such as mechanical strength, biotoxicity, biocompatibility, and biodegradability before research focus can switch to large-scale applications. Fabrication procedures need to be modified and improved in terms of facility and process parameters for better biomimicry and cost effectiveness. After further optimization of biomimetic, gradient, and 3D electrospun scaffolds along with the incorporation of advanced manufacturing techniques and novel materials, electrospun scaffolds exhibit substantial potential for cartilage tissue engineering.


## 5. Conclusion

This paper presents a variety of electrospinning strategies with novel materials and manufacturing techniques of bioscaffolds for cartilage tissue engineering. The literature review reveals that the most prevailing recent trend is the fabrication of biomimetic, gradient, and 3D bioscaffolds. Natural polymeric and biological materials have been incorporated into electrospinning technique with synthetic materials to improve biomimicry and biocompatibility. Multiple approaches have been taken in electrospinning to form 3D scaffolds with cartilage-like structure and enhanced chondrogenic differentiation. Mechanical properties of scaffolds have been improved by various electrospinning strategies to achieve acceptable levels. Future research should focus on issues such as mechanical strength, biotoxicity, and biodegradabilityin vivo to pave the way for possible human trials.



---

*Source: 1953636-2018-03-25.xml*